Research Article  Open Access
Dongliang Zhang, Xiaoyan Zhang, Yunrong Luo, Qingyuan Wang, "Experimental Study on DropWeight Impact Response of Basalt Fiber Aluminum Laminates (BFMLs)", Advances in Materials Science and Engineering, vol. 2018, Article ID 1478951, 13 pages, 2018. https://doi.org/10.1155/2018/1478951
Experimental Study on DropWeight Impact Response of Basalt Fiber Aluminum Laminates (BFMLs)
Abstract
The basalt fiberreinforced polymer (epoxy resin), which has even better mechanical properties than glass fiberreinforced polymer, is a good choice for making FML (fibermetal laminate) composite. Herein, dropweight impact tests of basalt fiberbased FMLs (called BFMLs) were conducted in the INSTON 9520HV testing machine to investigate the lowvelocity impact properties of BFMLs. The specimens were of two diameters. And the impactors had two sizes of nose, dropping from different heights. The loaddeflection behavior of aluminum sheet, BFRP (basalt fiberreinforced polymer) panel, and BFML plate and their energy dissipation patterns during impact perforation were obtained. The test results showed that aluminum alloy sheet and BFMLs had no strain rate effect, while BFRP did. It was also concluded that the behavior of the thick BFML plate was clearly affected by debonding between aluminum sheet and BFRP panel, while the behavior of the thin BFML plate was controlled by membrane force. In failure analysis, it was found that the deformation and breakage of BFRP are the main contributions to energy absorption of BFMLs which counts for more than 75%. The energy absorbed by the aluminum sheet through plastic deformation and petaling is about 20%, while the energy absorbed in debonding can be ignored. In addition, with the help of ABAQUS simulation, it was found that decreasing the value of MVF (metal volume fraction) can increase the specific energy absorption of BFMLs, but the ductility of BFMLs may decrease.
1. Introduction
Fibermetal laminates were firstly designed for aircraft structures [1, 2]. Highvelocity impact events are the main problems that FMLs mostly faced in aviation industry [1, 3]. Along with the expansion of applications of FMLs to land transportation from aviation industry, lowvelocity impact response of FMLs has been increasingly attracted attention since it quite often happens to vehicles on road [4–7].
Many researchers have studied lowvelocity impact behavior of FMLs such as GLARE, ARALL, CARALL, and hybrid FMLs using two kinds of fibers and/or particular metals like magnesium and titanium [8, 9]. From those studies, people gain more understanding on how FMLs react to impacting events. Therein, delamination is the distinctive feature of FMLs during lowvelocity impact. The deflection stiffness and energy absorption are closely related to delamination of FMLs, which also contributes to the complexity in analyzing mechanical behavior of FMLs [10, 11].
There are few articles discussing the fabrication of fibermetal laminates [12], but it is the prerequisite step before conducting the experimental study. Surface treatment of the metal layer can have significant effects on the interlaminar properties and thus the overall properties of FMLs. Thus, Aghamohammadi et al. [13] investigated four different surface treatment methods on the aluminum layers and studied their effects on the flexural behavior of FMLs. The effect of metal layer distribution on FMLs was concerned by Khan and Sharma [14, 15] in experimental and simulation ways. Norman Jones [16] made some theoretical predictions for the deformation and denting of fibermetal laminates when subjected to lowvelocity impact loads. The rigid plastic material approximation with modifications to reflect the actual cross section of a fibermetal laminate was used to produce simple formulae which gave reasonable agreement with the corresponding experimental data.
However, of fibers applied in all types of FMLs, basalt fiber is rarely reported. Continuous basalt fiber has been widely used in automotive industry due to its superior mechanical properties in comparison to Eglass fiber, which can be seen in Table 1 [17]. In addition, basalt fiber has flame retardancy and is able to maintain high performance at high and low temperatures [18, 19]. Basalt fiber also has high abrasive and corrosive resistance, which can be used in the detrimental environment [20, 21]. Also, basalt fiber is nontoxic to human body [22].

Since basalt fiber has so many advantages, it is a potential substitute of glass fiber in FMLs’ fabrication that may be used in automobiles. Thus, basaltbased FMLs were studied in this paper.
2. Preparation of Specimens
2.1. Materials
2A12T4 aluminum alloy sheets with a thickness of 0.5 mm were supplied by Southwest Aluminum (Group) Co., Ltd (China). The basalt fiberreinforced polymer (epoxy resin) with a thickness of 1.32 mm was supplied by Sichuan Aerospace Tuoxin Basalt Industrial Co., Ltd (China). The adhesive film made of modified polyethylene acrylate was supplied by Shanghai Zhenghuan Adhesive Product Co., Ltd (China). The chemical components and basic mechanical properties of 2A12T4 aluminum alloy are listed in Table 2 and Table 3, whilst the parameters of continuous basalt fiber (CBF) and its composite are listed in Table 4. Table 5 gives material properties of BFRP.




2.2. Specimen Design
A simple methodology was used to prepare BFMLs, with five steps listed as follows:(1)Materials were cut in the light of BFMLs’ size in order to avoid direct clipping on BFMLs which may introduce damage in interfaces between aluminum alloy sheet and BFRP layer.(2)Surface treatment was applied to both materials so as to improve bonding quality when using adhesive film. Polishing (abrasion) on BFRP surface aimed at increasing roughness which is beneficial to bonding quality, while chemical cleaning, including alkali wash, acid cleaning, and phosphoric acid anodizing of aluminum alloy sheet, was also applied for the same purpose.(3)Adhesive film (AF) was laid between aluminum alloy sheet and BFRP layer to make them initially bonded through hotrolling to form semifinished product of BFMLs.(4)Semifinished product of BFMLs was placed into moulds, with the applied pressure of 5 MPa and heat of 160°C, followed by a curing period of 60 minutes.(5)The specimen was aircooled.
3. DropWeight Impact Tests
The dropweight tests were conducted in the INSTON 9520HV testing machine, as shown in Figure 1. The acceleration transducer was mounted in the drop hammer to record the history of acceleration. Optical grating was mounted at underpart of a stand column to record the initial impact velocity of the projectile. After once and twice integrals of acceleration, the history of velocity and displacement of the projectile can be obtained. The reaction force between the projectile and the BFML specimen can be calculated by Newton’s second law. Moreover, the history of load, energy, velocity, and deflection during impact can also be obtained.
Aluminum alloy sheet and BFRP and BFML plates were tested by dropweight impact. The specimens were clamped between two square steel plates with a circular opening at the center, as shown in Figure 1. The opening of steel plates has two diameters, i.e., 70 mm and 100 mm. The projectile is of hemisphere with the diameters of 10 mm or 20 mm and masses of the projectile of 5.666 kg, 14.353 kg, or 17.493 kg. The heights of the drop weight were set as 0.36 m, 0.48 m, or 0.76 m.
4. Results and Discussion
4.1. StrainRate Effect
In most cases, stiffness and strength of a material may increase with strain rate. The strainrate effect during impact on a composite plate has a contribution to enhancing the bending stiffness and/or strength. While, if the loaddeflection curve of a material under impact is similar to that under static loading, there is no strainrate effect for such dynamic loading.
In order to investigate the strainrate effects of the aluminum alloy sheet, BFRP layer, and BFML plate, dropweight impact tests were conducted on the three types of materials, and the test results of dropweight impact are listed in Table 6.
 
^{1}20Al701 represents the testing condition as follows: projectile diameter is 20 mm, specimen material is aluminum sheet, specimen diameter is 70 mm, and serial number of specimen is 1. 
4.1.1. 2A12T4 Aluminum Alloy Sheet
According to Damith [23], aluminum alloy shows hardly any strainrate effect when the strain rate is less than 800 s^{−1}. As the strain rate on the aluminum alloy sheet by a dropweight impact in the present study is no more than 110 s^{−1}, the strainrate effect on the 2A12T4 aluminum alloy sheet was therefore ignored. Figure 2 shows the loaddeflection curves of 2A12T4 aluminum alloy sheets under dropweight impact. It can be seen that, in moderate strainrate regime, there was no significant difference between curves in the impact velocity regime of 2.63–3.70 m/s. As for the deviation of the static result from impact curves, difference of the corresponding global deflection may attribute to it. Response of the 2A12T4 aluminum alloy sheet under static loading is always global, while that under impact loading gave rise to more localized indentation in the vicinity of the impact region so that the stiffness of 2A12T4 aluminum alloy sheet bending under impact is somewhat higher than that under static loading during early stage, say, deflections less than 2 mm. Afterwards, the bending stiffness showed no difference between static and impact curves considering slope and peak load.
4.1.2. BFRP
The strain rate of the BFRP plate can be estimated by means of average impact velocity being divided by radius [24]. Although BFRP plates do show some strainrate effect, such effect in the range of 25–97 s^{−1} seems minimal, which almost covers the strain rate range in the present study, as shown in Figure 3. The bending stiffness and ultimate load carrying capacity of BFRP plates under impact are nearly twice of that under static loading. However, the peak load of BFRP plates under impact was independent of projectile’s diameter.
(a)
(b)
4.1.3. BFMLs
BFMLs showed no strainrate effect. Similar to the 2A12 aluminum alloy sheet, localized indentation is responsible for the higher initial bending stiffness, which explains why the initial segment (where deflection is less than 2 mm) of the loaddeflection curve of impact is steeper than that of static, as shown in Figure 4. Therefore, no strainrate effect of BFMLs is considered in prediction of impact behavior of BFMLs plates in Section 4.2.
4.2. LoadingDeformation Relationship of BFML Plates
When the loading rate was not high, such as dropweight impact, the analysis of dynamic behavior of structures may be converted to that of quasistatic process based on the modal analysis method [25].
2A12 aluminum alloy is an elasticplastic ductile material, while BFRP is a linear elastic brittle material. In order to obtain analytical expressions for the loaddeflection response of BFMLs, 2A12 aluminum is idealized as a rigid plastic material with linear strain hardening and BFRP is idealized as a linear elastic material, as shown in Figure 5.
4.2.1. Thin Plate
The principle of minimum potential energy was applied to derive the loaddeflection relation of thin BFML plates (type of 2/1 BFML plate).
The total strain energy of the BFML panel consists of bending and membrane energy. Since the inplane deformations are negligible compared to the transverse deflections, the strain energy can be expressed in terms of transverse deflections only.
For the symmetric BFML plate, the strain energies of aluminum alloy sheets and BFRP panels due to bending are given bywhere is the integral area, and are the fully plastic bending moments in x and y directions, is the twisting moment in the xy plane, and D_{ij} is the bending stiffness. The plastic bending and twisting moments can be derived by taking moments about the neutral surface of the plate which are expressed in the following equation:where is the number of aluminum sheets, is the distance of neutral surface of the aluminum sheet from that of the BFML plate, and is the thickness of the aluminum alloy sheet.
The membrane strain energies of aluminum alloy sheets and BFRP plates can be expressed by the von Kármán straindisplacement relations:where and are fully plastic membrane and inplane shear forces and is the membrane stiffness. The membrane and inplane shear forces can be obtained by taking stress resultants about the neutral surface of the plates which are expressed in the following equation:where is the yield strength of the aluminum alloy sheet.
The deformation profile of BFMLs needs to be considered when applying the principle of minimum potential energy. Tsamasphyros and Bikakis [26] proposed a velocity profile of GLARE panels under lowvelocity impact as
The deformation profile of BFMLs can be obtained by integrating the above equation:where is the radius of the BFML plate. Under symmetrical loading conditions, the inplane shear force and twisting moment are zero. By substituting Equation (8) into Equations (1), (2), (4), and (5), we can get the bending strain energy and membrane energy as follows:
The work of external load is
By calculating the minimal value of the potential energy,there iswhere
The deflection of the thin BFML plate (type of 2/1) was several times the thickness of the BFML plate, and thus membrane force is dominant in responding to external loading. By ignoring the bending force, the following expression can be obtained:
The theoretical prediction by Equation (17) is in a good agreement with the related test results, which is shown in Figure 6.
4.2.2. Thick Plate
The small deflection profile of the clamped circular plate under lateral loading was given by the classical theory of plates:where is the load, is the radius of the plate, and is the bending stiffness which is
The deflection at the center of loading can be obtained through Equation (18):
Therefore, the peak load is
The average elastic modulus of the BFML plate can be calculated bywhere is the hardening slope of 2A12 aluminum alloy and is the static elastic modulus of BFRP.
Figure 7 shows the predicted loaddeflection curves compared with the test results of 4/3 BFMLs. The test results began to deviate from the predicted curve which did not take debonding (dashed line) into account when the deflection was more than 1 mm. Debonding may occur even when the impact load on the BFML plate is well below the peak load, as shown in Figure 8, which reduces the bending stiffness of the BFML plate. Therefore, the effect of debonding on the BFML plate stiffness must be considered during dropweight impact. The debonding radius can be given in terms of the lateral load () and the interlaminar shear strength (ILSS) between aluminum alloy sheet and BFRP [26]:
The bending stiffness of debonding area, as shown in Figure 9, can be calculated bywherewhere i and j are the numbers of the aluminum alloy sheet and BFRP plate, respectively. The stiffness of bonding area is calculated by Equations (19) and (22). Then, the deflection composes of two parts ( and ) that are formed in bonding and debonding areas (Figure 9).
Figure 9 shows that the predicted loaddeflection curve after considering debonding is in a good agreement with the test results, which demonstrates that the behavior of the thick BFML plate is closely related to the debonding phenomenon. It was further analyzed in the case that there was no debonding occurred, as shown in Figure 10. When the debonding is not dominated in the BFML plate after dropweight impact, the predicted loaddeflection curve without considering debonding is more accurate than that considering debonding. It is worth pointing out that, in Figure 10, the initial bending stiffness of the loaddeflection curve (less than 0.5 mm of deflection) should be calculated based on the elastic modulus of 2A12 aluminum alloy rather than the hardening slope (E : E_{p} = 70.1 GPa : 1.5 GPa).
4.3. Failure Mode
The failure modes of the 2A12 aluminum alloy sheet and BFRP plate were both different on whether they are impacted alone or as components of BFMLs. The monolithic aluminum alloy sheet tends to form a plug during impact but petals during quasistatic loading as shown in Figure 11. The evident cross crack lines can be seen in loading area of the BFRP plate after static indentation while serious breakage was formed after impact as shown in Figure 12. As components of BFMLs, 2A12 aluminum alloy sheet and BFRP layer failed under impact were more like the way that both materials failed under static indentation, as shown in Figure 13. This means that the calculated energy based on static tests should be preferred in energy analysis of failure.
(a)
(b)
(a)
(b)
(a)
(b)
4.4. Energy Partition
The kinetic energy of the projectile was absorbed by global deformation of the BFML plate, debonding, fiber breakage, and plastic deformation and damage of 2A12 aluminum alloy during perforation. The energy balance equation is as follows:where is the total absorbed energy and , , and , are energies absorbed in debonding, tensile fracture of BFRP, deformation, and petaling of the 2A12 aluminum alloy sheet, respectively.
4.4.1. Energy Absorbed in Debonding
Debonding will propagate in mode II at a critical force [27]:where is Poisson’s ratio, is the plate stiffness, and is the mode II critical interlaminar shear fracture toughness. The radius of debonding area iswhere is the shear strength of interface which was obtained by conducting tensile shearing tests on bonding surface between aluminum alloy sheet and BFRP plate. In the present study, ILSS = 30.0 MPa.
Energy absorbed in debonding is
Combining Equations (27)–(29) gives
4.4.2. Energy Absorbed by BFRP
The fracture energy density of BFRP can be obtained based on the area under strainstress curve of the tension test, which is E_{t} = 2.85 × 10^{6} J/m^{3}. The fracture energy of the BFRP plate under static indentation can be calculated by making the product of energy density to tensile failure by the volume of primary fiber region, shown in Figure 14. The calculated fracture energy is nearly equal to the test results, as shown in Table 7. Therefore, the energy absorbed in tensile fracture of BFRP in BFMLs during impacting perforation is given bywhere is the number of BFRP layers, is the radius of projectile, is the radius of BFML plate, and is the thickness of the single BFRP layer.

The membrane energy absorbed by the secondary fiber area where no fiber breakage occurred was calculated by Equation (12).
4.4.3. Energy Absorbed by 2A12 Aluminum Alloy Sheet
Based on the previous analysis, the membrane strain energy of the aluminum alloy sheet in BFMLs can be expressed as
Taking as the maximum deflection of BFMLs, the plastic strain energy of the single aluminum alloy sheet can be obtained by
Furthermore, as the projectile perforating specimen, aluminum sheet bends back around projectile’s periphery. The plastic work in petaling of n layers iswhere is the number of aluminum alloy sheets and is the radius of the projectile.
Therefore, the energy partition of BFMLs is now clear, which is summarized in Table 8. The proportions of energy absorbed by constituent materials are shown in Figure 15. It can be seen that the energy absorbed by BFRP accounts for more than 75% of the total energy absorbed. The calculated total energy absorption is compared with the test results in Figure 16. Most of the calculated energies are in a good agreement with the test results. The reason for the discrepancies in the second and last ones may be due to the dispersiveness of ductility of the 2A12 aluminum alloy sheet as shown in Table 3.

If the total energy absorbed is divided by area density of the BFML plate, the specific energy absorption can be obtained. Figure 17 shows the specific energy absorption varies with metal volume fraction (MVF). The curves of MVF represent only the trends it varies. The two lines of MVF originate from two series of BFMLs, as shown in Figure 18. Series I was generated from numerical simulation using the commercial code ABAQUS (the corresponding properties such as absorbed energy were necessarily obtained from simulation in ABAQUS), while series II consisted of the specimens in the test. Both series of BFMLs (Figure 17) show that decreasing the MVF brings the higher specific energy absorption. However, the ductility of BFMLs is inevitably weakened with a low amount of ductile aluminum alloy.
5. Conclusions
Loaddeflection relationships of 2A12 aluminum alloy sheets, BFRP plates, and BFML plates under dropweight impact were obtained. The strain rate was calculated as impact velocity divided by specimen diameter, which was the averaged result over specimen span. It was used as an indicator in strainrate effect analysis. Its accuracy is not high, but it is a convenient way to qualitatively inspect strain raterelated properties. Only BFRP plates showed strainrate effect. As a result, dropweight impact behavior of BFML plates was analyzed based on the static indentation. Moreover, the failure modes of 2A12 aluminum alloy sheets and BFRP layers in BFML plates were more or less similar to those of both monolithic materials failed in static indentation. Therefore, the fracture energies of each material in BFML plates were calculated based on properties obtained in static tests.
Thin and thick BFML plates under impact behaved quite differently. The behavior of thin BFML plates is controlled by membrane stress, while the bending stiffness of thick BFML plates is dependent on debonding between aluminum alloy sheet and BFRP layer.
The energy absorbed by BFRP layers in BFML plates accounts for more than 75% of total absorbed energy, indicating that BFRP is the main energy absorbing material. Decreasing MVF can raise the specific energy absorption of BFML plates. However, there must be a limit of MVF for the guarantee of the necessary ductility.
Data Availability
The data used to support the findings of this study are included within the article.
Conflicts of Interest
The authors declare no conflict of interest.
Authors’ Contributions
Dongliang Zhang and Qingyuan Wang were responsible for the conceptualization. Dongliang Zhang and Yunrong Luo were responsible for the methodology. Xiaoyan Zhang was responsible for the software. Qingyuan Wang and Yunrong Luo were responsible for the funding acquisition.
Acknowledgments
This research was funded by the Changjiang Scholars and Innovative Research Team (IRT14R37), National Natural Science Foundation of China under Grant No.11572057, Talent Introduction Project of Sichuan University of Science and Engineering (2015RC34), and the Project of Key Laboratory of Material Corrosion and Protection of Sichuan Province (2016CL17).
References
 C. A. J. R. Vermeeren, “An historic overview of the development of fibre metal laminates,” Applied Composite Materials, vol. 10, no. 45, pp. 189–205, 2003. View at: Publisher Site  Google Scholar
 L. B. Vogelesang and A. Vlot, “Development of fibre metal laminates for advanced aerospace structures,” Journal of Materials Processing Technology, vol. 103, no. 1, pp. 1–5, 2000. View at: Publisher Site  Google Scholar
 G. H. Majzoobi, H. Morshedi, and K. Farhadi, “The effect of aluminum and titanium sequence on ballistic limit of bimetal 2/1 FMLs,” ThinWalled Structuers, vol. 122, pp. 1–7, 2018. View at: Publisher Site  Google Scholar
 Z. Asaee and F. Taheri, “Experimental and numerical investigation into the influence of stacking sequence on the lowvelocity impact response of new 3D FMLs,” Composite Structures, vol. 140, pp. 136–146, 2015. View at: Publisher Site  Google Scholar
 J. Bienias, P. Jakubczak, and K. Dadej, “Lowvelocity impact resistance of aluminium glass laminates – experimental and numerical investigation,” Composite Structures, vol. 152, pp. 339–348, 2016. View at: Publisher Site  Google Scholar
 J. Fan, W. Cantwell, and Z. Guan, “The lowvelocity impact response of fibermetal laminates,” Journal of Reinforced Plastics and Composites, vol. 30, no. 1, pp. 26–35, 2011. View at: Publisher Site  Google Scholar
 M. Sadighi, M. Y. Tooski, and R. C. Alderliesten, “An experimental study on the low velocity impact resistance of fibre metal laminates under successive impacts with reduced energies,” Aerospace Science and Technology, vol. 67, pp. 54–61, 2017. View at: Publisher Site  Google Scholar
 S. M. R. Khalili, A. Shokuhfar, K. Malekzadeh, and F. Ashenai Ghasemi, “Lowvelocity impact response of active thinwalled hybrid composite structures embedded with SMA wires,” ThinWalled Structures, vol. 45, no. 9, pp. 799–808, 2007. View at: Publisher Site  Google Scholar
 S. Zhu and G. B. Chai, “Lowvelocity impact response of fibremetal laminates–experimental and finite element analysis,” Composites Science and Technology, vol. 72, no. 15, pp. 1793–1802, 2012. View at: Publisher Site  Google Scholar
 S. J. L. Curiel and N. Karapurath, “Delamination modelling of GLARE using the extended finite element method,” Composites Science and Technology, vol. 72, no. 7, pp. 788–91, 2012. View at: Publisher Site  Google Scholar
 M. Kharazan, M. H. Sadr, and M. Kiani, “Delamination growth analysis in composite laminates subjected to low velocity impact,” Steel and Composite Structures, vol. 17, no. 4, pp. 387–403, 2014. View at: Publisher Site  Google Scholar
 D. W. Lee, B. J. Park, S. Y. Park, C. H. Choi, and J. I. Song, “Fabrication of highstiffness fibermetal laminates and study of their behavior under lowvelocity impact loadings,” Composite Structures, vol. 189, pp. 61–69, 2018. View at: Publisher Site  Google Scholar
 H. Aghamohammadi, S. Navid Hosseini Abbandanak, R. EslamiFarsani, and S. M. Hossein Siadati, “Effects of various aluminum surface treatments on the basalt fiber metal laminates interlaminar adhesion,” International Journal of Adhesion and Adhesives, vol. 84, pp. 184–193, 2018. View at: Publisher Site  Google Scholar
 S. H. Khan, A. P. Sharma, R. Kitey, and V. Parameswaran, “Effect of metal layer placement on the damage and energy absorption mechanisms in aluminium/glass fibre laminate,” International Journal of Impact Enginnering, vol. 119, pp. 14–25, 2018. View at: Publisher Site  Google Scholar
 A. P. Sharma, S. H. Khan, R. Kitey, and V. Parameswaran, “Effect of through thickness metal layer distribution on the low velocity impact responds of fiber metal laminates,” Polymer Testing, vol. 65, pp. 301–312, 2018. View at: Publisher Site  Google Scholar
 N. Jones, “Note on the impact behavior of fibremetal lamiantes,” International Journal of Impact Engineering, vol. 108, pp. 147–152, 2017. View at: Publisher Site  Google Scholar
 T. Deak and T. Czigany, “Chemical composition and mechanical properties of basalt and glass fibers: a comparison,” Textile Research Journal, vol. 79, no. 7, pp. 645–651, 2009. View at: Publisher Site  Google Scholar
 Q. Liu, M. T. Shaw, R. S. Parnas, and A. M. McDonnell, “Investigation of basalt fiber composite mechanical properties for applications in transportation,” Polymer Composites, vol. 27, no. 1, pp. 41–8, 2006. View at: Publisher Site  Google Scholar
 A. Ross, “Basalt fibers: alternative to glass?” Composite Technology, vol. 12, pp. 44–8, 2006. View at: Google Scholar
 B. Oztürk, F. Arslan, and S. Oztürk, “Hot wear properties of ceramic and basalt fibre reinforced hybrid friction materials,” Tribology International, vol. 40, no. 1, pp. 37–48, 2007. View at: Publisher Site  Google Scholar
 F. Rabinovich, V. Zueva, and L. Makeeva, “Stability of basalt fibres in a medium of hydrating cement,” Glass and Ceramics, vol. 58, no. 11/12, pp. 431–4, 2001. View at: Publisher Site  Google Scholar
 F. M. Kogan and O. V. Nikitina, “Solubility of chrysotile asbestos and basalt fibres in relation to their fibrogenic and carcinogenic action,” Environmental Health Perspectives, vol. 102, pp. 205–6, 1994. View at: Publisher Site  Google Scholar
 M. Damith, A. Muneeb, and N. Tuan, “Outofplane impact resistance of aluminum plates subjected to low velocity impacts,” Materials and Design, vol. 50, pp. 413–426, 2013. View at: Publisher Site  Google Scholar
 M. S. Mahmood and J. O. Majid, “Investigating the transverse behavior of glassepoxy composites under intermediate strain rates,” Composite Structures, vol. 93, no. 2, pp. 690–696, 2011. View at: Publisher Site  Google Scholar
 X. Yu, Shock Mechanics, Tsinghua University Press, Beijing, China, 2011.
 G. J. Tsamasphyros and G. S. Bikakis, “Dynamic response of circular GLARE fibremetal laminates subjected to low velocity impact,” Journal of Reinforced Plastics and Composites, vol. 30, no. 11, pp. 978–987, 2011. View at: Publisher Site  Google Scholar
 S. H. F. Michelle, C. Lin, M. R. Duane Jr., and D. A. Hopkins, “Ballistic impact of GLARE fibermetal laminates,” Composite Structures, vol. 61, no. 12, pp. 73–88, 2003. View at: Publisher Site  Google Scholar
Copyright
Copyright © 2018 Dongliang Zhang et al. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.